AB2-type monomers were synthesized, which made the solution present a light yellow color . The solution was transferred to an eggplant-shaped flask and put into an automatic rotary vacuum evaporator. After
evaporation of methanol under low pressure, the temperature was Combretastatin A4 chemical structure raised to 150°C using an oil bath to initiate the polymerization of the monomers. Eventually, a yellowish viscous multi-amino compound (RSD-NH2) was obtained with a 4-h polymerization. Preparation of the silver nanoparticles Silver nitrate (AgNO3) and the multi-amino compound (RSD-NH2) were dissolved in deionized water, separately. Then AgNO3 aqueous solution was added dropwise into the RSD-NH2 solution under vigorous stirring. AZD1480 The initial concentrations of the reaction components were 0.017, 0.085, 0.17, and 0.255 g/l for AgNO3 and 2 g/l for RSD-NH2. The reacting mixture was kept stirring at room temperature until reduction of Ag+ to Ag was completed and brown silver nanoparticles appeared. Characterization of the silver nanoparticles The size distribution and polydispersity of the silver nanoparticles were determined by MK5108 ic50 dynamic light scattering (DLS)
using a HPPS 5001 grain size analyzer (Malvern Instruments Ltd., Malvern, UK). Transmission electron microscopy (TEM) micrographs were obtained using a Tecnai G220 TEM (FEI Company, Hillsboro, OR, USA) operated at a 300-kV accelerating voltage. TEM samples were prepared by evaporating a drop of nanoparticle solution onto a 200-mesh copper grid, which was coated with a carbon support film. UV-visible (UV-vis) absorption spectra were recorded using an UV-3010 spectrophotometer (Shimadzu Ltd, Japan). K/S absorption spectra of treated silk fabrics were tested under a D65 illuminant at 10° observer using an Ultrascan XE spectrophotometer (HunterLab Co. Ltd., Reston, VA, USA). The X-ray
diffraction (XRD) patterns of the silver nanoparticles were taken in the 2θ range of 20° to 80° at a scanning rate of 2°/min using Cu Kα radiation with a model D/max3c X-ray detector diffraction system (Rigaku Ltd, Japan). For Fourier transform infrared (FTIR) analysis, the colloidal silver solution was poured into acetone only and the resulting precipitates were dried for characterization. FTIR spectra were performed on a Nicolet 5700 FTIR spectrophotometer (Thermo Electron Corporation, USA). Preparation of silver nanoparticle-treated silk fabrics The silk fabrics were immersed into the solution of mixed AgNO3 and RSD-NH2 at their respective concentration with the process of dipping and rolling twice. Subsequently, the fabrics were steamed for 30 min in a steam engine (BTZS10A, China). After that, the fabrics were washed by deionized water and dried at ambient temperature to produce the finished silk fabric.